### R E V I E W

### Open Access

## Modelling of Damage Evolution in Braided

## Composites: Recent Developments

### Chen Wang

1,2,3### , Anish Roy

2### , Vadim V. Silberschmidt

2### and Zhong Chen

1*Abstract

Composites reinforced with woven or braided textiles exhibit high structural stability and excellent damage tolerance thanks to yarn interlacing. With their high stiffness-to-weight and strength-to-weight ratios, braided composites are attractive for aerospace and automotive components as well as sports protective equipment. In these potential applications, components are typically subjected to multi-directional static, impact and fatigue loadings. To enhance material analysis and design for such applications, understanding mechanical behaviour of braided composites and development of predictive capabilities becomes crucial. Significant progress has been made in recent years in development of new modelling techniques allowing elucidation of static and dynamic responses of braided composites. However, because of their unique interlacing geometric structure and complicated failure modes, prediction of damage initiation and its evolution in components is still a challenge. Therefore, a comprehensive literature analysis is presented in this work focused on a review of the state-of-the-art progressive damage analysis of braided composites with finite-element simulations. Recently models employed in the studies on mechanical behaviour, impact response and fatigue analyses of braided composites are presented systematically. This review highlights the importance, advantages and limitations of as-applied failure criteria and damage evolution laws for yarns and composite unit cells. In addition, this work provides a good reference for future research on FE simulations of braided composites.

Keywords:Braided composite, Damage evolution, Finite-element model, Failure criteria, Mechanical behaviour, Impact behaviour, Fatigue

Introduction

Braiding is a method used to interweave two or more fibre yarns to produce textile composites. The angle between the longitudinal direction of a braided preform and bias yarns is generally defined as braiding angleθ; it ranges typ-ically from 15° to 75°. Both two-dimensional (2D) and three-dimensional (3D) braided architectures can be fabri-cated in many ways, such as two-step or four-step method of rectangular braiding, tri-axial braiding, circular braiding, and other displacement braiding techniques (Bilisik 2012). The main feature of a braided method is its flexibility to achieve variable geometric shapes with high volumes of parts in a cost-effective way. Thanks to the unique undula-tions of the braided structure, macro cracks have no clear path to grow in epoxy matrix, and their propagation can be arrested at inter-sections of yarns. As a result, braided

textile composites enjoy higher fracture toughness, struc-tural stability and better damage tolerance compared to pre-preg and laminated composites (Mouritz et al. 1999). With their high stiffness-to-weight and strength-to-weight ratios, braided composites are attractive materials for aerospace and automotive components as well as sports protective equipment (Ayranci and Carey 2008).

In order to enhance understanding of braided compos-ites, it is crucial to evaluate properties and predict their failure under static and dynamic loading. On the other hand, this topic is still quite challenging, considering com-plicated braided structures of such composites, rendering nonhomogeneous and anisotropic properties at the con-stituent level. Extensive efforts in analysis of braided textile composites have been made since 1980s, with most studies aimed at investigating their mechanical behaviour using analytical and/or experimental approaches. In analytical schemes, elastic constants of textile composites were esti-mated from homogenised equivalents of the representative unit cell (RUC) structure using the rule of mixtures. The

* Correspondence:ASZChen@ntu.edu.sg

1_{School of Materials Science and Engineering, Nanyang Technological}
University, 50 Nanyang Avenue, Singapore 639798, Singapore
Full list of author information is available at the end of the article

predicted levels of strengths were generally higher than those in experimental observations; these higher values were attributed to limitations of linear elastic assumptions in the analytical expressions (Naik and Shembekar 1992; Quek et al. 2003). On the other hand, experimental stud-ies were regarded as expensive and time-consuming. In addition, these studies did not have the capability to pro-vide stress and strain distributions throughout braided patterns or fundamental information on damage models inside the braided composites (Miravete et al. 2006; Littell et al. 2009a, b; Xu et al. 2015a). Thus, it became necessary to seek assistance of powerful computer-aided-design (CAD) and computer-aided-engineering (CAE) tools to clarify damage mechanisms of braided structures and to predict the ultimate strength of composites with such structures.

It is not easy to develop a reliable geometrical model to simulate real braided structures due to the interlacing of yarns and complexity of the braided geometry. One of the difficulties in modelling fabric composites is an inhomo-geneous distribution of fibre yarns in them. In some of the practical applications, in-plane properties of textile com-posites were treated as homogeneous. For instance, textile composites were represented by a composite shell (Xiao et al. 2011; Schwab et al. 2016) or layers of solid elements (Xiao et al. 2007; Yen 2002) and their stress-strain behav-iours were modelled with constitutive models developed for unidirectional (UD) or woven composites; obviously, the accuracy of these models for large-tow textile compos-ites was limited. A lack of consideration of a meso-scale structure in finite-element (FE) models was one of the rea-sons for such discrepancy. Therefore, a number of research teams implemented FE analysis of braided textile compos-ites based on meso-scale geometry models. In these at-tempts, a RUC was used to evaluate mechanical behaviour of the whole composite structures equivalently (Pankow et al. 2012; Cousigné et al. 2013; Wan et al. 2015).

Mesoscopic structures of braided composites can be rep-resented by various methods. A pioneering work was done by Lomov et al. (2001) who developed a software tool, WiseTex, for geometry modelling of internal structure of textile reinforcement, such as 2D/3D woven, bi-axial/tri-axial braided and knitted etc., transferring data into general FE codes. A similar work was carried out by a Textile Com-posites Research Group at the University of Nottingham in UK (Wong et al. 2006). A Python-based open-source

software, TexGen, combined geometry building with

volume-meshing algorithms. In addition, a well-known mosaic model and a sub-cell model (Aitharaju and Averill 1999) were developed. In the former, a compos-ite structure was discretised into a mosaic assemblage, with each mosaic brick element having distinct material properties. Global displacement or stress could be ap-plied to the macro level model and then transferred to

mosaic blocks using iso-stress or iso-strain conditions (Bogdanovich 2009). Sub-cell FE models considered a meso-structure of textile composites in terms of simpli-fied RUC representations. However, instead of being homogenized, the RUC was decomposed into three or four sub-cells, and their effective elastic constants were obtained by micromechanical analysis (Aitharaju and Averill 1999) employing equivalent (Zhou et al. 2013; Zhang et al. 2014a) or idealized laminate (Xiao et al. 2007). FE models for the RUCs were subsequently con-structed using solid elements of each set of property ac-cording to their locations in the RUC. Based on this approach, a generalized method of cells (GMC) was devel-oped (Qi et al. 2014; Bednarcyk et al. 2015). GMC con-siders a periodic repeating unit cell and is limited to four sub-cells (one for fibre and three for matrix). This theory was firstly generalised by Paley and Aboudi (1992) to con-sider an arbitrary number of sub-cells and constituent phases. The resulting GMC enables analysis of repeating unit cells containing more than two constituent materials, a more refined fibre shape, and various fibre architectures. Using GMC, Liu et al. (2011) built a framework for a three-scale analysis of tri-axially braided composites, and effective properties of the RUC at each scale were deter-mined. The advantages and shortcomings of these topo-logical meso-geometry models were pointed out by Fang and Liang (2011). The main advantage was that the meso-scale models obtained with these methods could be me-shed easily. However, this scheme faced the challenges of internal continuity and stress-singularity problems, which were caused by distinctive elastic properties of two adja-cent mosaic blocks (Dai and Cunningham, 2016). Also, realistic meso-geometrical configurations were ignored in the topological methods. Recently, virtual descriptions of the geometries of braided textiles were developed using 3D SolidWorks and CATIA (Ji et al. 2014; Wang et al. 2016b). These versatile geometric unit cells were highly flexible and dynamic in nature, capable of simulating tex-tile tightening, accommodated by yarn deformation and spatial constraint. The unit-cell geometries were then fed into FE analysis packages to determine their individual and continuum-mechanical characteristics (Ji et al. 2014).

for evaluation of the occurrence of material damage. With development of studies on damage mechanisms of com-posites, although multiple failure criteria for composites were suggested, even a most accepted failure criterion might not be suitable for all the conditions.

The degradation models are mathematical representa-tions of residual properties for each material damage state predicted with the failure criteria (Garnich and Akula, 2009). The most direct way for damage modelling is a fracture-mechanics-based approach, in which cracks are directly introduced into the model. Still, introducing cracks inside complex yarns-matrix architecture and re-meshing are computationally intensive. Continuum dam-age mechanics (CDM), which can provide a tractable framework for modelling damage initiation and develop-ment with a strategy of stiffness degradation, is one of the important and effective methods to model progressive damage behaviour of fibre-reinforced composites sup-ported by FE procedures. The main advantage of CDM is the straightforwardness with implementation into FE ana-lysis; since the material is continuous throughout the dam-age process, it does not require re-meshing (Murakami 2012). CDM provides not only the final failure load, but also information concerning the extent of integrity of the material during the load history.

Ansar et al. (2011) systematically reviewed the modelling techniques along with their capabilities and limitations for characterization of the micro-geometry, mechanical behav-iour and impact behavbehav-iour of 3D woven composites. A comprehensive literature survey was also conducted by Fang and Liang (2011) to review the methods of numerical analysis for 3D braided composites, including meso-scale modelling, mesh-generation techniques and progressive-damage models. These review papers indicated that although various damage degradation schemes based on

CDM were suggested, a universal model of damage mechanics, accounting for different loading conditions, fail-ure modes, damage initiation and evolution, is still lacking.

In order to improve efficiency and accuracy of simula-tion work, scientists continued to develop various state-of-the-art damage-evolution methods for braided composites in past few years. Based on the review works by Ansar et al. (2011) and Fang and Liang (2011), the objective of this paper is to review recent developments made in failure analysis of braided composites. Most of the studies discussed herein were published after 2011. The contents are organised as follows: First, acceptable failure criteria and advanced damage-evolution models for predicting mechanical response of braided composites are discussed. Then, recent numerical studies on impact behaviour are introduced. Last but not least, modelling strategies of fatigue damage are provided.

Review

Criteria for failure initiation

A typical progressive-damage model (PDM) comprises three parts: stress analysis, failure analysis and material-property degradation (Zhou et al. 2013). These parts are implemented in an iterative procedure performed until the final failure occurs. The stress analysis is linked to appropriate constitutive relationships for both undam-aged and damundam-aged materials, which requires adequate damage-initiation criteria revealing main failure mecha-nisms and compatible with FE models. A specific damage-evolution model is needed to describe material-property degradation after damage initiation. To date, the failure criteria, applied predominantly to braided composites, are still developed from classical damage the-ories of laminated composites. Garnich and Akula (2009) reviewed some of the most commonly applied criteria for UD fibre-reinforced polymers and classified them into either mode-dependent or mode-independent criteria.

Nowadays, two categories of failure criteria are actively pursued. Mode-independent failure criteria use mathem-atical expressions to depict a damage surface as a func-tion of strength of materials. All the polynomial and tensorial criteria belong to such a category. Tsai-Wu criteria are the most well-known and general one for composites, belonging to a type of Tensor Polynomial Criterion (Tsai and Wu 1971). For practical proposes, the polynomial criterion is expressed in tensor notation as (Hart-Smith, 1998)

FiσiþFijσiσj≥1; ð1Þ

wherei,j= 1…6. The parametersFiandFijare related to
the composite strength in the principal directions.
Con-sidering that failure of the material is insensitive to a
change of sign in shear stresses, all terms containing a
shear stress to first power must vanish:_{F}4=F5=F6= 0.

Then, the explicit form of the general expression is:

F1σ1þF2σ2þF3σ3þ2F12σ1σ2þ2F23σ2σ3

þ2F13σ1σ3þF11σ21þF22σ22þF33σ23≥1:

ð2Þ

In recent studies, the Tsai-Wu tensor polynomial failure criterion was used by McLendon and Whitcomb

(2012) and Wang et al. (2017b) to identify, which loca-tion (s) in the tows are the first to fail under a given loading. Jiang et al. (2013) modified this criterion consid-ering an additional bending stress and the interaction force between curved yarns to determine longitudinal strength of 3D braided composites under a uniaxial load. Cousigné et al. (2013) applied the Tsai-Wu criterion to predict mechanical failure of woven composites and mentioned that the criterion offered a smooth continuous ellipsoidal failure surface efficiently without involving specific and complex failure modes, as shown in Fig. 2. Wan et al. (2015) used Hill’s anisotropic plasticity model to predict failure of fibre tows. Hill’s potential function is a simple extension of the Mises function, which can be expressed in terms of rectangular Cartesian stress compo-nents. Besides the Tsai-Hill criterion (1968), several other similar quadratic criteria have been proposed by Hoffman (1967) and Chamis (1969). These criteria can be consid-ered as generalized Tsai-Wu type criteria.

Traditional ply-based failure criteria, such as Tsai-Wu and Tsai-Hill, consider a yarn-matrix system as a whole and, therefore, they are not suitable to predict whether the failure occurs inside a yarn, a matrix, or at their interfaces (Tolosana et al. 2012). When characterising failure of com-posites, researches focus on their homogeneity rather than anisotropic nature. This is inappropriate since internal unique structures of composites influence their properties and failure character (Paris and Jackson 2001). Moreover, the polynomial criteria may be not suitable in design, particularly for bi-axial tensile loading (Edge 2002). Considering a non-homogeneous character of braided composites, mode-dependent criteria were proposed.

Mode-dependent criteria are generally established in terms of mathematical expressions based on material strengths. They consider different failure modes of the constituents. Because of this advantage, these criteria are adequate for PFA. Two of the simplest examples are the maximum-stress and maximum-strain criteria. The former criterion predicts that composites fail when the stress exceeds the maximum tolerance value. Three different conditions of failure are considered for a maximum stress in a longitudinal direction, a transversal direction and for shear stresses:

Longitudinal:

σ1≥XTorj jσ1≥XC; ð3Þ

Transverse:

σ2≥YTorj jσ2≥YC; ð4Þ

Shear:

τ12≥S12orjτ23j≥S23; ð5Þ

In Eqs. (3)–(5),XTandYTdenote tensile strengths in the

longitudinal (X) and transverse (Y) directions of a braided

composite, respectively. XC and YC are compressive

strengths in the X and Y direction of the composite, re-spectively. Indices 1, 2 and 3 are used to describe X, Y and Z directions, respectively. Hence, S12, S13 and S23 signify in-plane and two out-of-plane shear strengths, respectively. The effective normal and shear stress component are denoted byσiandτij(i,j= 1 , 2 , 3 ;i≠j), respectively.

Similarly, the maximum-strain criterion means that when the strain exceeds the given allowable value, the constitutive materials fail. These maximum criteria can be used for homogeneous textile composite models (Sevkat et al. 2009a, b). As simple methods to analyses composites failure, the major limitation of the maximum-stress and maximum-strain criteria is that they ignore the interaction between stresses and strains in the composites. Therefore, they were mostly applied to specific constitutive material elements, such as failure of fibre (Mao et al. 2013), yarns (Dai and Cunningham, 2016) or pure matrix resin (Sun et al. 2013; Qi et al. 2014).

In contrast, some mode-dependent failure criteria take into account interactions between stresses and strains (they are called interactive failure criteria), including Hashin (1980), Puck and Schürmann (1998) and micro mechanics-based failure (MMF) criteria (Ha et al. 2010). Hashin proposed different failure modes associated with the fibre tow and the matrix, considering, in both modes, differences in tension and compression (Hashin 1980), as shown in Fig. 3. The values of initiation damage criteria

∅Ifor each type of failure modeIare as follows:

Fibre tensile failure in longitudinal direction ∅t

L: (σ1≥0)

∅t L¼

σ1

XT

2

þφ½α τ212

S12

ð Þ2þα τ2

13

S13

ð Þ2 ¼1; ð6Þ

Fibre compressive failure in longitudinal direction

∅c

L: (σ1< 0)

∅c L¼

σ1

XC

2

¼1; ð7Þ

Matrix tensile failure in transverse direction ∅t

Y: (σ2+σ3≥0)

∅t Y ¼

σ2þασ3

YT

2

þατ223−σ2σ3

S23

ð Þ2 þ

τ2 12

S12

ð Þ2þα

τ2 13

S13

ð Þ2¼1;

ð8Þ

Matrix compressive failure in transverse direction ∅c_{Y}:
(σ2+σ3< 0)

∅c Y ¼ YC 2S23 2 −1 " #

σ2þασ3 YC

þ σ2þασ3

2S23

2

þατ223−σ2σ3 S23 ð Þ2

þ τ212 S12 ð Þ2þα

τ2 13 S13 ð Þ2¼1:

ð9Þ

In Eqs. (6)–(9), a plane-stress factor in each mode is

represented with α. When the through-thickness stress

component is ignored,α= 0. Otherwise, in a 3D case,α= 1. In the tensile fibre failure criteria, the coefficient φ is employed to determine the contribution of shear stress to the initiation of fibre tensile failure. The planar Hashin’s failure criteria with CDM degradation models controlled by energy-dissipation constants are implemented in ABAQUS, but only available for shell elements. Li et al. (2011) and Zhang et al. 2014, 2015a, b) applied the planar Hashin’s method to predict mechanical behaviour of braiding structures. In order to use 3D elements in ABAQUS, the Hashin’s 3D failure criteria were usually implemented in a user-defined subroutine (Warren et al. 2016; Zhang et al. 2017a). When the braided composites were regarded as orthotropic materials, failure modes in the thick-ness direction, as shown below, should be considered (Kang et al. 2016):

Matrix tensile failure in thickness direction∅t

Z(σ3≥0):

∅t Z¼

σ3

ZT

2

þσ23

S23

þ τ213

S13

ð Þ2¼1; ð10Þ

Matrix compressive failure in thickness direction ∅c

Z (σ3< 0):

∅c Z¼ σ3 ZC 2 þσ23 S23

þ τ213

S13

ð Þ2¼1: ð11Þ

In Eqs. (10) and (11), ZT and ZC denote tensile and

compressive strengths in the through-thickness (Z) dir-ection of a braided composite, respectively. In some studies, criteria for thickness-direction failure modes were presented in other forms (Fang et al. 2009; Zhou et al. 2013).

because, on the one hand, a linear criterion underesti-mated strength of the material and, on the other hand, a polynomial of higher degree would be too complicated to manage (Hashin 1980; Paris and Jackson 2001). Although Hashin himself limited the scope of his proposal to UD composites, the criteria were widely applied to braided composites in recent years (Binienda 2012; Zhang et al. 2014a; 2014b; Zhou et al. 2013).

So far, the mode-dependent failure criteria were proved to be more suitable for analysis of failure initi-ation in braided composites. Comparing to the Hashin’s failure criteria, even more failure modes were consid-ered in some studies. Doitrand and Fagiano (2015) applied an advanced failure criterion including different damage mechanisms such as fibre failure, transverse and out-of-plane cracking for the yarns, and inter-yarn-matrix cracking to study mechanical behaviour of a four-layer plain-weave glass fibre/epoxy matrix com-posite at the mesoscopic scale. It should be noted that the mode-dependent failure criteria can be also

presented in a based form, e.g. the Hashin strain-type criteria and a Linde criterion (Lu et al. 2013; Zhang et al. 2016a).

Micro-mechanics of failure is a theory that links con-stitutive materials (individual fibre, matrix and their interface) and a macroscopic stress response of compos-ites (Ha et al. 2008). It is believed that failure of fibrous composites can be assessed with micro-scale analysis. No difference between tension and compression failure modes at constituent levels is considered, and failure of fibre-matrix interface is incorporated:

fibre failure:

XC<σ1<XT; ð12Þ

X6

i¼1

X6

j¼1Fijσiσjþ

X6

i¼1Fiσi¼1; ð13Þ

matrix failure:

σ2

VMises CmTm

þ 1

Tm−

1

Cm

I1¼1; ð14Þ

interface failure:

tn h i

Yn

2

þ ts

Ys

2

¼1: ð15Þ

A fibre is a transversely isotropic material, and two possible failure criteria are needed for its failure. The first is a simple maximum-stress criterion; the other is the Tsai-Wu criterion. It was argued that the adoption of quadratic failure criteria, such as the Tsai-Wu, required the values of transverse tensile and compressive as well as shear strengths, which were diffi-cult to obtain in experiments. So, a simplification of the quad-ratic criteria to the maximum-stress criteria was preferred (Ha et al. 2010). The epoxy matrix is regarded as isotropic, and has a higher strength value under uniaxial compres-sion than under tencompres-sion. For the matrix, a Christensen Cri-terion was applied, which is a modified version of the von Mises failure criterion (Christensen 2007). Finally, the fibre-matrix interface can be considered to follow a traction-separation failure criterion (Ha et al. 2008, 2010).

MMF has gradually gained credibility as evident in the recent Second World-Wide Failure Exercise (WWFE II). MMF was reported to be able to predict successfully both the initial and final failures for all the 12 specified test cases (Kaddour and Hinton 2012). MMF is different from conventional methods primarily in two ways. On the one hand, the conventional methods are the ply-level failure methods while MMF is based on the constituent’s failure. On the other hand, the conventional macro-level methods generally require one or more interaction parameters in order to capture the interaction of stress components in the matrix and fibres, while MMF uses a micromechanical model to account for the stress interaction, so that the inter-action parameter is not needed (Xu et al. 2015a, b). A modi-fied MMF scheme was proposed to improve predictions of shear strength by adding shear component in the criteria

(Ha et al. 2010). In addition, since σ11 component was

closely related with fibre failure, it was assumed thatσ11did not contribute to matrix failure. Thus, the MMF scheme was simplified to three-parameter MMF (MMF3):

1

Tm−

1

Cm

σ22þσ33

ð Þ þ 1

TmCmðσ22þσ33Þ

2

− 1

S2m

σ22σ33− τ2

12þτ223þτ231

¼1

ð16Þ

Damage mechanics

To model progressive failure of braided textile com-posites, numerous studies combined two

damage-evolution theories for inter- and intra-laminar dam-ages, respectively. The first theory was a cohesive zone model (CZM), widely used to capture inter-laminar delamination (Xie et al. 2006). Application of CZM requires a-priori knowledge of an intended crack path and a use of cohesive elements. Another theory to evaluate intra-laminar failure was con-tinuum damage mechanics (CDM) (Camanho et al. 2003; Heinrich et al. 2013). In CDM, damage is de-scribed by introducing internal state variables (Dij)

into an algorithm of continuum mechanics to repre-sent micro defects in a damage process in the mater-ial. Stiffness values of composites degraded with the

growing damage variables (DVs) Dij homogeneously

when a material met its failure criteria. Therefore, post-peak behaviour of materials can be described by

a degraded stiffness matrix C(Dij) or compliance

matrix S(Dij) as

σ

ij¼C Dij εijorεij¼S Dij σij;i;j

¼1;2 and 3;respectively: ð17Þ

Although many methods were developed, it is still an open question how to define DVs considering complicated failure modes of braided composites. In this section, some stiffness-degradation approaches most broadly used in recent investigations are discussed.

Instantaneous stiffness degradation

An instantaneous stiffness-degradation method was initially developed by Blackketter et al. (1993) and Matzenmiller et al. (1995). In this empirical stiffness-reduction scheme, DVs are usually constants. When stresses at an integration point of a finite element satisfy the damage-initiation criterion, damage at this integration point happens and stiffness is reduced to a specific value according to the relevant failure mode. The scheme was widely used for damage prediction in composites without any convergence difficulties. It also showed good cap-ability to simulate the mechanical performance of non-crimp fabric (NCF) composite structural parts associ-ated with different failure modes of yarns subjected to tension loading (Tserpes and Labeas, 2009). A degrad-ation factor associated with particular failure mode was used to multiply the corresponding modulus as soon as that particular mode of failure was detected. The com-puted damage initiation and accumulation had consist-ent results with experimconsist-ents. However, the results indicated that the final failure load depended on the mesh size and time increment.

analysis of carbon-fibre-reinforced woven composites. Microscale damage modes of the composite material were determined by using the maximum-stress criter-ion for fibres and the MMF for a matrix. The mech-anical response was assumed to be linear elastic until

initiation of failure. The instantaneous

stiffness-degradation method was applied, as shown in Fig. 4. For an element that reached the failure criterion, the elastic constants were reduced as follows:

Edij¼ 1−ð1−nÞ 1−dij

E0ij;i;j

¼1;2 and 3;respectively; ð18Þ

where Edij are the effective residual material properties

of the failed element,E0ijare the values of initial stiffness.

The softening factor n is computed to control the soft-ening process. In addition, dij are the degradation factors, prescribed in terms of reduction of effective stiff-ness along different directions. Failure analysis was carried out to provide the influence of each damage mechanism on overall laminates stiffness, and, thus,

the values of dij were determined by means of meso-mechanical failure analysis with six cases of boundary conditions. Additionally, quantitative analysis based on virtual tests was conducted to determine the deg-radation factors for every damage mechanism to con-trol the stress reduction in the damage-evolution law. The reported degradation factors are listed in Table 1.

Warren et al. (2016) developed a 3D progressive-damage model to capture the onset and initial propa-gation of damage in a 3D woven composite in a single-bolt, double-shear joint. The model combined the well-established Hashin failure criteria and the Matzenmillere-Lublinere-Taylor damage model to cap-ture bearing damage; failure indicators were used to calculate DVs. In this model, DVs affected directly elastic properties of the material by means of modifi-cation of diagonal components of a compliance matrix at each material point. For brittle materials, four DVs and all functions of the specific failure indi-cators, as seen in Table 2, were used to modify this material compliance matrix:

S dð Þ ¼

1

1−d1S11 S12 S13

0 0 0

S12

1

1−d2S22 S23

0 0 0

S13 S23

1 1−d2S33

0 0 0

1 1−d3S44

0 0

sym 1

1−d3S55

0

1 1−d4S66 2 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 5

ð19Þ

Its off-diagonal terms remained unaffected by DVs in order to satisfy physical and thermodynamic conditions. A similar method was applied by Wang et al. (2016a) to predict tensile strength of bi-axial braided composites with various braiding angles (Fig. 5), while studies by Ahn and Yu (2016) and Zhong et al. (2017) focused on a bending response of braided composites. Nobeen et al. (2016) stated that the appropriate reduction factors should be selected for the pure matrix and yarn damage of braided composites based on results of experiments and micro-mechanical numerical simula-tions. And such DVs (Eqs. (18) and (19)) were imple-mented in ABAQUS using the UMAT and USDFLD subroutines, respectively. They were stored as Solution

Dependent Variables and can be monitored throughout the progression of the analysis.

Although reasonable numerical results were obtained using the instantaneous stiffness-degradation method in many works, magnitudes of the stiffness-reduction factors were somewhat arbitrarily chosen by researchers based on the types of failure criteria and different failure modes. Therefore, the advanced failure criteria and dam-age factors for braided composites need to be investi-gated further, and more efforts are unquestionably needed in the future.

Continuous stiffness degradation

Evolution of DVs in the continuum stiffness-degradation method is based on a thermodynamic framework or an energy-dissipation theory. In the early stage, CDM was built to study damage development for single-ply or laminate composites because the damage mecha-nisms of UD composites were relatively easy to quantify. Nowadays, various evolution laws based on the continuum stiffness-degradation method are also suitable for braided composites. In these studies, the evo-lution of DVs could be presented in a linear or an expo-nential form.

When constituents of a material fail in an element, it dissipates energy equal to its elastic energy. According to an approach by Lapczyk and Maimí (Lapczyk and Hurtado, 2007; Maimí et al. 2007), a characteristic elem-ent length was introduced into an expression to solve a mesh-dependence problem. The equivalent displacement at failure pointXf

eq is defined as follows:

Xfeq ¼εIfl; ð20Þ

where l is the characteristic length of the element and

εIf is the equivalent strain at failure of failure mode I. Thus, degradation of the stiffness tensor is character-ized by a damage matrix,C(D), defined by internal DVs

dI associated to different failure modes I (Fang et al.

2009). When the Hashin failure criteria are applied, the DV of each failure mode is expressed by the following equivalent displacement:

dI ¼X If

eq XIeq−XIieq

XIeq XIfeq−XIieq

ðI¼Lt;Lc;Yt;Yc;Zt;ZcÞ: ð21Þ

Figure 6 shows the linear evolution of DVs. Accordingly, XIieqand XIfeqin Eq. (21) are the initiation and full damage

equivalent displacements of failure modeI, respectively. XIieq and XIfeq could be calculated with the following

equations (Kang et al. 2016):

Table 1Degradation model for all damage mechanisms

(Mao et al. 2013)

Degradation factor Matrix failure Matrix failure in weft yarn Matrix failure in warp yarn Fibre failure in weft yarn Fibre failure in weft yarn

d11 0.75 1 0.85 0.001 1

d22 0.75 0.85 1 1 0.001

d33 0.001 0.25 0.25 0.85 0.85

d12 0.01 0.25 0.25 0.001 0.001

d23 0.01 0.75 0.25 0.25 0.001

d13 0.01 0.25 0.75 0.001 0.25

Table 2Definition of damage variables in Warren et al. (2016)

Damage mode Damage variable value

Pure matrix phase dm= 0.9

Longitudinal damage (fibre) d1¼

0:93 tesnion 0:8 compression

Transverse damage (matrix)

d1¼

0:86 tesnion 0:6 compression

Longitudinal shear (combined) d3= 1−(1−d1)(1−d2)

XIieq ¼
X_{ﬃﬃﬃﬃﬃﬃ}Ieq

∅I

p ; ð22Þ

XIfeq ¼

2GI

σIi eq

: ð23Þ

Here, ∅Iis the value of damage-initiation criteria. GI

and σIi

eq are the fracture energy density and the initiation
damage equivalent stress of failure mode I, respectively.
The initiation equivalent stress σIi_{eq} could be calculated
from the following equation:

σIi eq¼

σI eq

ﬃﬃﬃﬃﬃﬃ

∅I

p : ð24Þ

In Eqs. (21)–(24), the equivalent stress σI_{eq} and the
equivalent displacement XIeq associated to different failure

modes are expressed in Table 3. The equivalent displace-ments of damage initiation listed in Table 3 have the similar forms with Eq. (21).

Therefore, the damage-evolution equation is associated with the characteristic element length, local strain and fracture energy of the braided-composite constituents. The damaged stiffness matrixC(D) can be expressed in a matrix form by using the components of undamaged stiff-ness matrix and the principal values of the damage tensor

DI according to the Murakami-Ohno damage model

(Murakami, 1988).

In the studies conducted by Li et al. (2011), the pro-cesses of local damage propagation and failure of braided composites were quantified using the above bilinear dam-age evolution law. Local failure mechanisms, such as fibre splitting and matrix cracking, were taken into consider-ation. In a FE model, the braiding architecture of the fibre tows was modelled at meso-scale. Fang and Liang (2011) investigated the compressive properties of 3D braided composites using this damage theory. The material’s dam-age in damdam-aged stiffness matrixC(D) was computed with three internal DVs that were characterizing fibre, matrix and shear damage (df,dmandds, respectively):

C Dð Þ ¼_{Δ}1

1−df

E1 1−df

1−dm

ð Þυ21E1 0 1−df

1−dm

ð Þυ12E2 ð1−dmÞE2 0 0 0 ð1−dsÞG12 2

6 4

3 7 5;

ð25Þ

where Δ= 1−(1−df)(1−dm)υ12υ21. In these studies,

only planar stress components were considered, other-wise, a fully three-dimensional damaged stiffness matrix was developed as

Fig. 5Predicted stress-strain curve of bi-axial braided composites and damage contours (Wang et al. 2016a)

where Δ′= 1−dfdmυ12υ21−dmυ23υ32−dfυ13υ31−2dfdmυ21

υ32υ13. Zhang et al. 2014, 2015a, b) applied such 3D dam-aged stiffness matrix with the mentioned equivalent stress and displacement relationship to investigate the contribu-tion of local details of the braiding architecture and the local stresses, strains, and damage mechanisms on the glo-bal response of braided composites. In Zhang’s studies, a fully three-dimensional FE model was developed, with peri-odic boundary conditions applied along the gauge section length, and free boundary conditions applied at the two free edges of the model of the experimental coupon. The model also showed the capability of predicting a free-edge effect besides the primary damage evolution in tri-axial braided composites, as shown in Fig. 7.

Zhou et al. (2013) implemented a two-step, multi-scale progressive-damage analysis to study damage and failure behaviours of 2D plain weave composites under various uniaxial and biaxial loading conditions. In this model, a similar bilinear damage evolution approach (Zako et al. 2003) with a formal-unified 3D Hashin-type criterion were employed to facilitate analysis and engineering applications, with shear nonlinearity considered in the stiffness matrix of yarn. The results showed that tensile strength decreased for off-axis angles (see Fig. 8). In the Zhou’s study, the damaged stiffness matrix could be presented explicitly as follows:

C Dð Þ ¼ b2

LC11 bLbTC12 bLbZC13 0 0 0

b2TC22 bTbZC23 0 0 0

b2ZC33 0 0 0

sym bLTC44 0 0

bTZC55 0

bZLC66

2 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 5 ;

ð27Þ

where bL= 1−DL, bT= 1−DT, bZ= 1−DZ,

bLT¼ 2 1ð2−−DDLLÞð−1D−TDTÞ

2

, bTZ¼ 2 1ð2−−DDTTÞ−ð1D−ZDZÞ

2

, bZL¼ 2 1ð2−−DDZZÞ−ð1D−LDLÞ

2

.

Cij (i,j= 1 , 2 , 3) are the components of the undamaged stiffness matrix,DL,DTandDZare the DVs in longitudinal, transverse and thickness directions, respectively, based on Eq. (21). Such a scheme was also applied by Zhang et al.

(2015a) to study meso-scale progressive damage of 3D

five-directional braided composites under transverse compression.

The linear damage-evolution method was also adopted by Matveev et al. (2014) combined with a voxel mesh technique to analyse variability of fibre strength numer-ically from micro to macro-scale taking into account the size effect and transitions between the scales. The multi-scale approach demonstrated that a wide distribution of fibre strength led to a narrow distribution of composite strength accompanied a shift to lower mean values.

Another multi-scale approach for PFA of braided com-posites at coupon-level was elaborated and validated by Xu et al. (2015a, b). Starting from elastic constants of con-stituents (i.e. fibre and matrix), ply-level effective material properties were predicted using a micro-mechanical unit-cell model, with ply’s effective properties assigned to each tow in a meso-mechanical model of braided composites. In their study, the damage evolution was determined by the equivalent strain, a scalar measure of the strain com-ponents. Using the equivalent strain and equivalent stress, a multi-linear stress-strain damage model was proposed for the matrix in fibre tows, as illustrated in Fig. 9.

As shown in Fig. 9, the mechanical response of yarns followed the linear stress-strain relation before damage occurred in the matrix. After this, the material exhibited

C Dð Þ ¼Δ′

1−dmυ23υ32

ð ÞdfE11 ðυ21þυ23υ31ÞdfdmE11 ðυ31þυ21υ32ÞdfE11 0 0 0

1−dfυ13υ31

dmE22 υ32þdfυ12υ31

dmE22 0 0 0

1−dfdmυ12υ21

E33 0 0 0

sym dfdmG12 0 0

dmG23 0

dfG31

2 6 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 7 5

; ð26Þ

Table 3Equivalent displacements and stresses corresponding to different failure modes

Failure modeI Equivalent displacement Equivalent stress

Lt,σ1≥0 XLteq¼l

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

<ε11>2_{þ}_{ε}2
12þαε231

p

lð<σ11><ε11>þσ12ε12þασ13ε13Þ=XLt_{eq}

Lc,σ1< 0 XLceq¼l<−ε11> lð<−σ11><−ε11>Þ=XLc_{eq}

Yt,σ2≥0 XYteq¼l

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

<ε22>2_{þ}_{ε}2
12þαε223

p

lð<σ22><ε22>þσ12ε12þασ23ε23Þ=XYt_{eq}

Yc,σ2< 0 XYceq¼l<−ε22> lð<−σ22><−ε22>Þ=XYc_{eq}

Zt,σ3≥0 XZteq¼l

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

<ε33>2_{þ}_{ε}2
23þε231

p

lð<σ33><ε33>þσ23ε23þσ13ε13Þ=XZt_{eq}

Zc,σ3< 0 XZceq¼l<−ε33> lð<−σ33><−ε33>Þ=XZc_{eq}

hardening behaviour followed by softening, depending on the damage state. In order to predict the strength, meso-scale FE models of representative unit cells of bi- and tri-axial braided composites were developed (Xu et al. 2015a, b). Another example was presented by Zhao et al. (2016) to bypass the complexity associated with meso- and

micro-mechanics. They proposed simplified methods for progressive-failure prediction in braided composites mainly subjected to uniaxial in-plane loading and bending. The global stress-strain behaviour and principle damage modes in bending were obtained without losing much accuracy.

Apparently, most schemes were based on linear dam-age models. A non-linear damdam-age evolution approach Fig. 7Free-edge warping behaviour:aout-of-plane displacement;bscheme of warping locations and directions (Zhang et al. 2015a, b)

Fig. 8Strength of woven composites for different off-axis angles

was first proposed by Maimí et al. (2007) to regularize the energy dissipated at a material point by each failure mechanism. A viscous model is usually applied to mitigate the convergence difficulties associated with strain-softening constitutive models. Therefore, the non-linear damage evolution law is usually presented as an expo-nential expression in the following general form:

di¼1− 1

f rið Þexp½Aið1−f rið ÞÞ; ð28Þ

where the subscript i denotes different damage modes,

di, f(ri), Ai and ri are the DV, the damage-activation function, the coefficient and the damage threshold value, respectively. In recent investigations, the non-linear damage evolution approach was applied to capture pro-gressive damage evolution in braided composites in static and quasi-static loading regimes.

Lu et al. (2013) determined a set of reasonable inter-facial properties for predicting a mechanical response of 3D braided composites under uniaxial tension and inves-tigated the effect of interfacial properties on their stress-strain behaviour. In their numerical model, a 3D Linde failure criterion was adopted to describe a progressive-damage process in yarns, which was a strain-based con-tinuum damage formulation with different failure criteria for fibre and matrix failure modes, respectively. A grad-ual degradation of the material properties was assumed, which was controlled by the individual fracture energies of fibre and matrix. Failure occurred once effective strain f(εi) exceeded its threshold strain valueεif;t. DVs for fibre (df) and matrix (dm) modes were defined as follows:

df ¼1− εL f;t

fð ÞεL

exp −C11εLf;t fð ÞεL −εLf;t

_{L}

Gf

; ð29Þ

and

dm¼1− εT

f;t

fð ÞεT

exp −C22ε_{T}f;t fð ÞεT −εTf;t

_{L}

Gm

;

ð30Þ

where Gf and Gmare the fracture energy of the fibre and

matrix while L∗ is the characteristic length related to the elements. After failure initiation, the damaged stiffness matrix could be defined as

where dm1 and dm2 are two components of dm in

dif-ferent defined directions. To improve the convergence of nonlinear numerical calculations, a Duvaut-Lions viscous model (Duvaut and Lions 2012) was

imple-mented in UMAT. Therefore, the DVs di could be

regularized as:

_

Di ¼_{η}1ðdi−DiÞ ð32Þ

Here,ηis the viscous parameter andDiis the

regular-ized DV for each failure mode. Computing with this damage-evolution approach, the tensile modulus and strength of 3D braided composites were obtained with a good agreement to the experimental data. The calculated results showed that the effect of interfacial elastic modu-lus on the tensile modumodu-lus of 3D braided composites was prominent, while the strength of braided composites was not very sensitive to that parameter, as shown in Fig. 10.

Zhong et al. (2015) further developed the above mentioned exponential evolution approach for failure analysis of 3D woven composites under tension. Ex-cept for the longitudinal tension failure modes, the exponential damage evolution laws were still adopted for the fibre yarn in the model. Meanwhile, the linear and exponential damage evolution laws were used to represent the phenomena of fibre bridging and fibre pull-out in a fibre yarn (Bazant and Planas, 1997; Maimí et al. 2007), as shown in Fig. 11. The Puck failure criteria (Puck et al. 2002) were adopted for the fibre yarn as it could predict not only location but also orientation of a crack.

The damage process was irreversible, and the mech-anical properties degraded as soon as any criterion was activated. The DVs of the fibre yarn could be expressed as

d1t ¼1−

1−d1lt r1et

exp A1t 1−re1t

; ð33Þ

and

dN¼1− 1

rN exp½ANð1−rNÞ;N

¼f1c;2t;2c;3t;3cg; ð34Þ

C Dð Þ ¼C−

dfC11 dfþdm1

C12=2 dfþdm2

C13=2 0 0 0

dm1C22 ðdm1þdm2ÞC23=2 0 0 0

dm2C33 0 0 0

sym dfþdm1

C44=2 0 0

dfþdm2

C55=2 0 dm1þdm2 ð ÞC66=2 2

6 6 6 6 6 6 6 6 6 6 6 4

3 7 7 7 7 7 7 7 7 7 7 7 5

where AN is the parameter that defines the exponen-tial softening law. re1t, A1t and dl1t are the auxiliary

damage threshold parameter, the softening-law par-ameter and the DV for the longitudinal failure mode in tension, respectively. These parameters were de-fined by other material-property inputs. The DVs d4

and d6 represent the effect of damage on shear stiffness

due to fibre and inter-fibre fracture, andd5due to

inter-fibre fracture. So, the DVsd4,d6andd5could be given by:

d4¼1−ð1−d1Þð1−d2Þ; ð35Þ

d6¼1−ð1−d3Þð1−d1Þ; ð36Þ

and

d5¼1−ð1−d2Þð1−d3Þ: ð37Þ

Accordingly, S(d) is the damaged compliance matrix

of fibre yarns, which could be written as:

S dð Þ ¼ 1 1−d1 ð ÞE11 −

υ12 E11 −

υ13 E11

0 0 0

1 1−d2 ð ÞE22

−υ23

E22

0 0 0

1 1−d3 ð ÞE33

0 0 0

sym 1

1−d4 ð ÞG12

0 0

1 1−d5 ð ÞG23

0

1 1−d6 ð ÞG31

2 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 4

3 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 5

:

ð38Þ

The failure modes of the matrix are different from those of the fibre yarn. However, the exponential evolu-tion law could also be adopted based on mechanical response of the matrix material. Using this method, as seen in Fig. 12, the predictions of failure of woven com-posites under tension agreed well with the correspond-ing experiments (Zhong et al. 2015). The obtained results showed that mechanical properties of 3D woven composites were influenced by their thickness. The slope of stress-strain curve and the failure strength increased with the thickness growing.

Other advanced studies of progressive failure

Although complexities of modelling mechanical behav-iour of braided composites are present in many aspects, the improvement of modelling techniques is generally driven by two purposes. One is to account for all the physical phenomena observed in experiments in FE modelling; the other is to resolve numerical limitations of the FE method and balance its efficiency and accuracy.

Recently, nonlinear problems of mechanics of textile composites were considered in many studies. In experi-mental observations, two reasons of nonlinearities can be identified: a geometrical nonlinearity caused by a fabric structure and a material nonlinearity caused by micro-cracks evolving in the material inducing a loss of stiffness, indicating that the nonlinearity is related to progressive failure of the material. As mentioned above, the CDM approach generally uses a damage parameter Fig. 10Effect of interfacial elastic modulus on stress-strain curves of

3D braided composites (Lu et al. 2013)

characterizing the damage evolution responsible for the loss of stiffness due to micro-cracks. Besides, the nonlin-earity can be considered as macroscopic behaviour of the material independently from damage evolution.

Cousigné et al. (2013) developed a nonlinear numerical material model for textile composite materials consider-ing post-failure damage. The nonlinearity was repre-sented by the Ramberg-Osgood formulation. This formulation was developed by Bogetti et al. (2004) to estimate an equivalent stress function corresponding to an equivalent strain state:

σ¼ Eε

1þ Eε σa

_{n}

1

n;

ð39Þ

whereσais the asymptotic stress level andnis the shape parameter. The nonlinear behaviour was linked to a unidimensional plasticity definition to account for per-manent deformation without coupling between different material directions. Failure was predicted using the maximum-stress or Tsai-Wu failure criterion. A smeared formulation involving DVs was used to avoid undesirable localization phenomena (Pinho et al.2006). In this study, the model represented nonlinear material behaviour very well; a good agreement between experimental and nu-merical results was obtained under tensile and compres-sive loadings. However, the permanent deformation was still too high and stiffness degradation for the unloading process should be developed.

With development of the multi-scale modelling

approach, another key problem for improving the accur-acy of FE simulations is a link between micro- and

scale models. In a multi-scale approach, micro- and meso-scale models are usually carried out subsequently. Outputs of the microscopic model, including effective material properties of yarns, are commonly regarded as inputs for the meso-scale model (Šmilauer et al. 2011). In some stud-ies (Xu et al. 2015a, b; Mao et al. 2013), a correlation be-tween mesoscale tow stresses and microscale constituent stresses was established with the concept of a stress ampli-fication factor (SAF). The correlation can be expressed by the following formula:

σi¼MiσþAiΔT; ð40Þ

where σ and σi are the mesoscopic stresses and the microscopic stresses in fibres or matrix. The SAFs for the meso stressMiand for the temperature incrementAiwere determined by means of direct finite-element analysis of a micro-scale unit cell with proper boundary conditions. Similarly, Schultz and Garnich (2013) proposed a multi-continuum technology (MCT) and successfully predicted the initial matrix failure of a 0°/±45° tri-axially braided composite. The MCT provided a way to link the results provided by the meso-scale and macro-scale models with a good computational efficiency. In this approach, con-stituent properties were used to obtain composite proper-ties employing a micromechanical model. Then, an analytical relationship between composite stresses and strains and those in constituents was obtained based on an assumption that a continuum field existed for each constituent. This study also demonstrated capability of predicting initial matrix failure in textile composites with

nconstituent based on extension of the MCT.

Moreover, both micro- and meso-scale models can be developed with the GMC method. A comparison of meso- and micro-scale approaches to modelling progres-sive damage in plain-weave-reinforced polymer-matrix composites was carried out by Bednarcyk et al. (2015). As illustrated in Fig. 13, the meso-scale approach treated the woven composite tows as effective materials, utilizing an anisotropic continuum damage model. The micro-scale approach utilized the GMC semi-analytical micromecha-nical theory to represent a nonlinear response of the tows. The same damage model was used to model the matrix material within the tows. FE predictions were made for the shear and tensile responses of the plain-weave com-posite. Very similar results were obtained using the two approaches, for both effective behaviour of the woven composites and local damage fields predicted. For example, in the tensile simulations, both approaches predicted similar additional local damage coupling in the tow cross-over regions due to the multi-axiality of the stress fields. However, the FE results were considerably mesh-dependent because of softening present in the dam-age model. This mesh-dependence could be reduced with a crack-band approach, which regularized the energy dissi-pated in the damage model.

Recently, more advanced studies of mechanical proper-ties of 3D braided composites were considered to include some microscopic effects, such as defects. Dong and Huo (2016) developed a two-scale FE model for fibre tows and 3D braided composites to predict their elastic properties and micro stresses. Two basic types of defects - voids in a resin matrix and dry patches in fibre tows -were taken into account. The obtained results showed that the volume fraction of voids in fibre tows had a more notable effect on the elastic constants than those of the matrix. The longitudinal Poisson’s ratios increased with increasing volume fraction of voids, proving that presence of defects promoted transverse deformation in 3D braided compos-ites under longitudinal loading. However, the effect of internal defects on the strength was not included.

Döbrich et al. (2016) paid attention to a micro-scale character of a reinforcing textile in their study of a meso-scale RUC; this is not common due to higher

computational efforts compared with multi-scale

approaches. In this study, a digital element approach was used to model the textile structure with a near micro-scale resolution for the purpose of reinforcement

analysis. The textile unit-cell generation method

enabled a process-dependent modelling and, therefore, textile-specific simulations of composites with excellent agreement with real manufactured samples. Conver-gence analyses were carried out, and the textile model was directly used to build up a virtual composite model suitable for virtual mechanical tests, as illustrated in Fig. 14. A comparison of simulation results and test data demonstrated their very good agreement. The introduced model had a capability to be a part of a complete virtual process chain for development of high-performance composites.

To summarise, FE-based methods showed their cap-abilities and advantages in predicting the mechanical re-sponse of woven and braided composites. Numerous failure criteria and damage-evolution laws can be effect-ively applied in models of braided composite. Based on the above discussions, the main purpose of recent stud-ies was to improve simulation accuracy, which depends on two important considerations. The first one is that various failure modes observed in experiments should be accounted for in the FE simulations. The other is that advanced analytical approaches should be carried out to connect scales in multi-scale models. However, taking these considerations inevitably reduces the computational efficiency. Although some modelling attempts showed good accuracy when compared with experimental results, usually they were only demonstrated for a single structure or applicable only to some specific cases. More studies are needed to analyse the effect of braiding parameters, boundary conditions and complicated loading conditions in the future.

Modelling impact behaviour of braided composites During manufacturing, service life-time, maintenance etc., braided composites are often subjected to various dynamic loading conditions, from low-velocity impacts to ballistic loads. In such regimes, small weak point in a composite part can lead to catastrophic consequences. Therefore, a response of braided composites to such conditions should be clearly understood. An overview of general impact be-haviour of fibre-reinforced polymeric composites (FRPC) is given in some review papers (Davies and Olsson 2004; Crookston et al. 2005; Dixit and Harlal 2013). In most studies, the composites were impacted at different veloci-ties, and the resulting damage was evaluated. The effects of various parameters such as impact energy and impactor shape on impact responses of composites were also stud-ied. However, little attention was paid to braided compos-ites. Impact damage in structural textile composites was introduced into consideration recently (Binienda, 2012; Ma and Gao, 2013), and most of these efforts were based on experimental studies, rather than numerical simula-tions. This section introduces some recent numerical attempts to predict damage in braided composites under impact loadings, with impact energy from relatively low levels to high ones.

Modelling low-velocity impact of braided composites In a low-velocity impact (LVI), contact duration between an impactor and a target is long enough for entire struc-ture to respond and, hence, absorb more elastic energy. Low-velocity impacts with sufficient energy can cause various types of barely visible impact damage (BVID), such as matrix failure, delamination, fibre breakage, fibre-matrix debonding and fibre pull-out. The CDM ap-proach was investigated extensively in recent years and its application to impact-damage modelling proved to be very effective for UD laminates. Compared with lami-nates, few authors focused on a LVI response of woven and braided composites. LVIs are commonly encoun-tered in personal sports protection and some other structural fortifications.

The maximum-stress criterion with the instantaneous stiffness-degradation method was successfully used in modelling LVIs in braided composites. Sun et al. (2013) studied low-velocity impact properties of four-step 3D braided composites suffering a drop-weight impact with

velocity ranging from 1 m/s to 6 m/s. In this FE-based approach, impact damage was determined by maximum-stress criteria in several failure modes. In addition, the Critical Damage Area (CDA) theory introduced by Rosen (1964) and Hahn (1973) was also employed. The

CDA is governed by a composite’s interaction length,

which can be as low as 1 mm for tape-based composites and up to 100 mm for some 3D interlock weaves (Cox et al. 1996). According to the CDA theory, a critical damage length (δ) is defined as:

### δ

### ¼

### 4

### γ

_{f}

### X

f### 4

### τ

_{m}κ

κþ1

### ð

### κ

### þ

_{1}

### Þ

_{L}

### 2

### γ

_{f}

### "

### #

1κþ1

### ;

ð41Þwhereγfis the fibre-tow radius,Xfis the average tension strength of fibres,Lis the tow length, typically assumed 1 unit length, τm is the matrix yield stress, and κis the Weibull parameter, assumed to be 7.6. By definition, the critical damage area isδ2. As the damage area increases, the modulus of the fibre tows degrades as

Ei¼Ei0 1−

DA−DAif CDA

!2

" #

; ð42Þ

whereEiis theE11Young’s Modulus at pointi. Ei_{0} is the

undamaged modulus. CDA is the critical damage area.

DAis the area, where the value of longitudinal stress ex-ceeds the tension strength of the compositeXT, andDAif

is the value of DA when point i exceeds its maximum stress.DAis the next status ofDAif.

The instantaneous stiffness degradation scheme is shown in Table 4. The user-defined subroutine VUMAT is usually used to define the mechanical constitutive re-lationship of the 3D braided composite under drop-weight impact. VUMAT also works on failure

assess-ment and updates stress in ABAQUS. In the Sun’s work,

model predictions of a load-displacement curve, a peak force and energy corresponding to the peak force were in a reasonable agreement with experimental results. The damage morphologies of 3D braided composite specimens showed that the main failure mode was resin cracks, debonding and fibre-tow breakage.

fibre/unsaturated polyester resin composites with a con-ical impactor (Sun et al. 2012a, b). The corresponding load-displacement histories and failure modes were obtained from numerical simulation and verified by experimental results. It was observed that as the impact energy increased, both the maximum impact load and deflection also increased. Sevkat et al. (2009a, b) adopted a very similar approach to simulate drop-weight tests of hybrid plain-woven glass-graphite fibres/toughened epoxy composites with commercial 3D dynamic nonlinear FE software, LS-DYNA. Evolution of dynamic force, strain and absorbed energy as well as post-impact damage pat-terns obtained from experiments and FE simulations were in a good agreement. Colombo and Vergani (2016) char-acterized a textile carbon-fibre-reinforced composite in undamaged and damaged conditions, with numerical and analytical micromechanical approaches, in order to provide a method for assessing its residual stiffness after impact. An extent of degradation of the damaged compos-ite was estimated by Blackketter-type reduction factors applied to elastic properties of unit cells. The results showed that the values of the experimental in-plane residual stiffness in the damaged region decreased to 46% of its initial value. With this simple general approach, it was possible to predict a range of stiffness reduction for braided composites. However, in these studies, neither progressive damage nor plastic effect was accounted for in the FE models. Besides, values of the maximum impact displacement and interface delamination were not well captured. Usually, such approaches do not aim to run explicit simulations of the impact.

Continuous stiffness degradation associated with the Hashin failure criteria was also applied to dynamic prob-lems. Since this approach may lead to excessive element distortions and other related numerical difficulties, elem-ent deletion was utilised in simulation. Gideon et al. (2015) investigated a response of plain-woven basalt-unsaturated polyester composites to low-velocity impact both experimentally and with FE method simulations. Schwab et al. (2016) studied a carbon fabric/epoxy

system. In these studies, damage and failure behaviours of the textile composites was modelled using an ortho-tropic energy-based CDM approach, with DVs depend-ing on an equivalent stress-displacement relationship, as presented in Section 2.2; while delamination between layers was simulated with an interface cohesive-zone model. The simulations showed that a stress distribution during the impact event depended mostly on the reinfor-cing phase of the laminates. The behaviour of composites under low-velocity impact was defined mainly by the ini-tial impact energy, rather than impact velocity or impactor mass. The proposed modelling strategy provided the abil-ity to predict the overall energy absorption of a composite subjected to a transverse impact as well as energy contri-butions of individual mechanisms. Furthermore, shell elements were applied in these models to increase compu-tational efficiency and stability. Hence, these approaches were suitable to simulate complete perforation of the composite, as shown in Fig. 15. However, damage and failure within shell elements representing individual plies resulted from in-plane stress and strain components only. Therefore, damage due to transverse shear and out-of-plane tension was not accounted for. A comparative study was carried out by Wang et al. (2017a, Mater Des, under review) applying three-dimensional continuum and shell elements to explore the effect of through-thickness failure modes on energy absorption of the composite. In this study, a multi-scale computational approach was devel-oped and the 3D Hashin damage criteria were applied to capture main damage modes of a braided textile compos-ite. The results show that both surface- and element-based CZM can be applied as interface between composite layers. When shell elements were used as composite plies, the absorbed energy was underestimated. The progressive failure model with 3D stress elements provided more pre-cise results for the delamination areas and energy dissipa-tion capacity, at a higher computadissipa-tional cost.

In most of the modelling studies, the applied strategies provided a good representation at a homogeneous level, but could not represent the local damage modes related Table 4Failure criteria and degradation character according to Sun et al. (2013)

Failure Criteria Degradation

Tension along 1-direction σT

11>XT;CDA1>CDA E11= 0,G12= 0,G13= 0

Compression along 1-direction σC

11<XC E11= 0.95E11,σC11¼XC

Tension along 2-direction σT

22>YT E22= 0,G12= 0,G13= 0

Compression along 2-direction σC

22<YC σC22¼YC

Tension along 3-direction σT

33>YT E33= 0,G13= 0,G23= 0

Compression along 3-direction σC

33<YC σC33¼YC

Shear in 2–3 plane σS

23>SS23 G23= 0

Shear in 1–2 plane σS

12>SS12 G12= 0

Shear in 1–3 plane σS

to the weaving and braiding patterns. Pascal et al. (2015) described an extension of a semi-continuous approach in order to take into account the weaving pattern geom-etry. In this model, ply bundles were represented by 1D rod elements connected by nodes to 4 edges of a quadri-lateral shell element. Properties of the rods were adapted to represent local strain concentration. For delamination modelling, each ply was connected with a shell-to-shell interface element with a cohesive law. The main as-sumption about the damage mechanism was as follows: when resin was damaged, the local structure was lost and the ply’s bending stiffness was affected. The bundles were temporally and locally relaxed until, carrying all the loads, they failed in tension. Matrix failure was modelled with DVs for each local fabric directiondi (i=

1 and 2). d1affects E1and G13 while d2affects E2and

G23. These variables were functions of the energy-release rates Yi (i= 1 and 2), calculated from bending strains

and the Poisson’s ratio of the resin material. Damage

evolution was given by

di¼

ﬃﬃﬃﬃﬃ

Yi p

− ﬃﬃﬃﬃﬃﬃY0

p

þ ﬃﬃﬃﬃﬃﬃ

Yc

p if di<1

1 otherwise

i¼1;2

ð Þ

8 > < >

: ; ð43Þ

where Y0controls the damage initiation,Yc the damage evolution. ﬃﬃﬃﬃﬃYi

p

− ﬃﬃﬃﬃﬃﬃY0

p

þdonates positive part of the differ-ence between ﬃﬃﬃﬃﬃYi

p

and ﬃﬃﬃﬃﬃﬃY0

p

. Besides, a third

independent DVd12was implemented to model the final in-plane shear rupture. The bundle rupture in tension was assumed to be brittle. Therefore, the classic maximum-tensile strain criterion was used for rupture of the rods. In order to avoid numerical instabilities, when the maximum strain criterion was reached, the rod’s normal force F11 was smoothly decreased by the use of a characteristic timeτas follows:

F11¼F11 1−exp

t−t

τ

; ð44Þ

where t∗ is the exact time at which the criterion is reached andF11 the force stored at timet∗. Comparisons

with experimental data from drop-weight and gas-gun tests showed good accuracy of the force history and damage size and shape. As shown in Fig.16, the model-ling strategy was able to capture complex macro-crack paths observed experimentally as well as micro-cracking and delamination in the resin. With the numerical simu-lations, the influence of microstructure parameters on the impact behaviours could be revealed and the micro-structure could be optimized.

although the advanced strategy was able to represent local strain and stress fields related to the interlacing braided and woven architectures, it could hardly be used for large-scale structures.

High-velocity and ballistic impact

Different from a drop-weight scenario, the kinetic energy of a projectile under ballistic impact is observed to dissi-pate in the form of distinctive mechanisms. The pre-dominant energy absorption mechanisms of laminates under high-velocity impact are related to kinetic energy of moving a cone formed on a distal side of the target, frictional losses during penetration and energy absorp-tion related to failure modes, such as shear plugging, tensile fibre failure of primary yarns, fibre debonding, fibre pull-out, matrix cracking (intra-laminar) and inter-laminar delamination. For braided composites, although advanced numerical models were employed to predict their mechanical properties and failure modes, some of them are not suitable to study their ballistic behaviour because of high strain rates and high pressure conditions in the impact area in high velocity-impacts. It is well known that carbon/epoxy composites exhibit significant strain-rate sensitivity under such conditions.

Qiao et al. (2008) reviewed topics of impact mechanics and computational modelling of impacts (such as FE method, mesh-free methods and peri-dynamics). In their review, constitutive models of strain rate-dependent polymeric composites and their implementation in micromechanics models were briefly introduced. They also developed a nonlinear finite-element code (e.g., LS-DYNA) for impact and failure analysis. At an early stage,

the main purpose of modelling the ballistic response of composites was not their damage-evolution mechanisms. Instead, research was mostly aimed at macro ballistic parameters including residual velocities and maximum levels of dynamic displacement (Gower et al. 2008). Specifically, in terms of textile composites, the focus was on different composite features (like a fabric type and its

multi-layer structure), projectile geometry, impact

velocity and effect of friction of fabric yarns on the response of composites (Zeng et al. 2006; Rao et al. 2009a). Therefore, analysis of failure mechanisms still remains challenging in terms of accuracy of results and efficiency of the methodology.